data_zvyaginite 
_publ_contact_author_name    'Elena Sokolova'
_publ_contact_author_address     
'Dept Geological Sciences, University of Manitoba, Winnipeg, Manitoba, Canada'
_publ_contact_author_email       elena_sokolova@umanitoba.ca
loop_
_publ_author_name
_publ_author_address
'Elena Sokolova'
'Dept Geological Sciences, University of Manitoba, Winnipeg, Manitoba, Canada'
'A. Genovese'
'Environmental Sciences Div, King Abdullah University, Thuwal, Saudi Arabia'
'A. Falqui'
'Environmental Sciences Div, King Abdullah University, Thuwal, Saudi Arabia'
'Frank C. Hawthorne'
'Dept Geological Sciences, University of Manitoba, Winnipeg, Manitoba, Canada'
'Fernando Camara'
'Dipartimento di Scienze della Terra, Universita di Milano, Milano, Italy' 


_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
zvyaginite 
; 
_chemical_name_common             zvyaginite 
_chemical_formula_sum 
 'H9.11 Al0.07 Ca0.09 F0.89 Fe0.04 K0.04 Mn0.17 Na1.87 Nb1.68 O21.11 Si41.01 Ti1.25 Zn0.88' 
_chemical_formula_weight          812.17 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Na'  'Na'   0.0362   0.0249 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Si'  'Si'   0.0817   0.0704 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ti'  'Ti'   0.2776   0.4457 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Zn'  'Zn'   0.2839   1.4301 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Nb'  'Nb'  -2.0727   0.6215 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mn'  'Mn'   0.3368   0.7283 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Al'  'Al'   0.0645   0.0514 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'F'  'F'   0.0171   0.0103 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ca'  'Ca'   0.2262   0.3064 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            triclinic 
_symmetry_space_group_name_H-M    'C-1' 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 'x+1/2, y+1/2, z' 
 '-x, -y, -z' 
 '-x+1/2, -y+1/2, -z' 
 
_cell_length_a                    10.769(2) 
_cell_length_b                    14.276(3) 
_cell_length_c                    12.101(2) 
_cell_angle_alpha                 105.44(3) 
_cell_angle_beta                  95.17(3) 
_cell_angle_gamma                 90.04(3) 
_cell_volume                      1785.3(6) 
_cell_formula_units_Z             4 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     6840 
_cell_measurement_theta_min       2.38 
_cell_measurement_theta_max       30.06 
 
_exptl_crystal_description        plate 
_exptl_crystal_colour             creamy 
_exptl_crystal_size_max           0.004 
_exptl_crystal_size_mid           0.060 
_exptl_crystal_size_min           0.120 
_exptl_crystal_density_meas       2.88 
_exptl_crystal_density_diffrn     3.02 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              1578 
_exptl_absorpt_coefficient_mu     3.40 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.9288 
_exptl_absorpt_correction_T_max   0.9815 
_exptl_absorpt_process_details    'Bruker SADABS' 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'rotating-anode generator' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   Area 
_diffrn_measurement_method        ω 
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             10111 
_diffrn_reflns_av_R_equivalents   0.0457 
_diffrn_reflns_av_sigmaI/netI     0.0682 
_diffrn_reflns_limit_h_min        -14 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -19 
_diffrn_reflns_limit_k_max        19 
_diffrn_reflns_limit_l_min        -16 
_diffrn_reflns_limit_l_max        16 
_diffrn_reflns_theta_min          2.38 
_diffrn_reflns_theta_max          30.06 
_reflns_number_total              5101 
_reflns_number_gt                 3586 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0488P)²+138.6533P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        0 
_refine_ls_number_reflns          5101 
_refine_ls_number_parameters      340 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.1227 
_refine_ls_R_factor_gt            0.0923 
_refine_ls_wR_factor_ref          0.2368 
_refine_ls_wR_factor_gt           0.2207 
_refine_ls_goodness_of_fit_ref    1.089 
_refine_ls_restrained_S_all       1.089 
_refine_ls_shift/su_max           0.045 
_refine_ls_shift/su_mean          0.002 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
MH1 Nb 0.89893(9) 0.18624(8) 0.74159(10) 0.0196(4) Uani 0.891(7) 1 d P . . 
MH2 Nb 0.39831(9) 0.19855(8) 0.74170(10) 0.0183(4) Uani 0.877(7) 1 d P . . 
MO1 Ti 0.25277(19) 0.00006(14) 0.0013(2) 0.0223(6) Uani 0.975(12) 1 d P . . 
MO2 Na 0.2500 0.2500 0.0000 0.031(5) Uani 0.48(3) 2 d SP . . 
MO3 Na 0.7500 0.2500 0.0000 0.034(5) Uani 0.50(3) 2 d SP . . 
MO4 Zn 0.00009(13) 0.11964(10) 0.00036(15) 0.0199(5) Uani 0.817(8) 1 d P . . 
MO5 Na 0.4999(4) 0.1296(3) -0.0001(3) 0.0346(14) Uani 1.29(2) 1 d P . . 
AP1 Na 0.3928(5) 0.9354(5) 0.7030(6) 0.027(2) Uani 0.72(2) 1 d P . . 
AP2 Na 0.108(2) 0.072(3) 0.300(3) 0.101(19) Uani 0.27(3) 1 d P . . 
Si1 Si 0.1508(2) 0.8427(2) 0.7663(3) 0.0193(7) Uani 1 1 d . . . 
Si2 Si 0.1502(3) 0.0534(2) 0.7667(3) 0.0195(7) Uani 1 1 d . . . 
Si3 Si 0.1504(3) 0.3426(2) 0.7637(3) 0.0201(7) Uani 1 1 d . . . 
Si4 Si 0.3497(3) 0.9475(2) 0.2373(3) 0.0204(7) Uani 1 1 d . . . 
O1 O 0.5235(7) 0.2853(6) 0.7115(8) 0.0303(19) Uani 1 1 d . . . 
O2 O 0.7706(8) 0.2784(7) 0.7273(9) 0.037(2) Uani 1 1 d . . . 
O3 O 0.1555(7) 0.8798(6) 0.9056(7) 0.0254(17) Uani 1 1 d . . . 
O4 O 0.1602(8) 0.9367(5) 0.7140(8) 0.0281(18) Uani 1 1 d . . . 
O5 O 0.2696(8) 0.0994(7) 0.7291(9) 0.037(2) Uani 1 1 d . . . 
O6 O 0.0225(8) 0.0841(7) 0.7131(9) 0.037(2) Uani 1 1 d . . . 
O7 O 0.1548(7) 0.0778(6) 0.9057(8) 0.0257(17) Uani 1 1 d . . . 
O8 O 0.0222(8) 0.2810(7) 0.7272(9) 0.036(2) Uani 1 1 d . . . 
O9 O 0.2675(8) 0.2842(7) 0.7108(9) 0.038(2) Uani 1 1 d . . . 
O10 O 0.3264(8) 0.1187(6) 0.0975(8) 0.0286(18) Uani 1 1 d . . . 
O11 O 0.3691(8) 0.0640(6) 0.2893(8) 0.0297(19) Uani 1 1 d . . . 
O12 O 0.3262(8) 0.9243(6) 0.0992(8) 0.0281(18) Uani 1 1 d . . . 
O13 O 0.5224(8) 0.0963(6) 0.7270(9) 0.037(2) Uani 1 1 d . . . 
O14 O 0.7665(8) 0.0859(7) 0.7082(9) 0.040(2) Uani 1 1 d . . . 
XM1 O 0.9170(7) 0.2050(7) 0.8942(8) 0.032(2) Uani 1 1 d . . . 
XM2 O 0.4184(8) 0.2458(7) 0.8953(8) 0.034(2) Uani 1 1 d . . . 
XA1 O 0.3821(7) 0.9780(6) 0.9072(8) 0.0280(18) Uani 1 1 d . . . 
XA2 O 0.0986(7) 0.0199(6) 0.0888(7) 0.0226(16) Uani 1 1 d . . . 
XPM1 O 0.8882(12) 0.1537(10) 0.5424(10) 0.056(3) Uani 1 1 d . . . 
XPM2 O 0.3713(11) 0.1405(10) 0.5431(10) 0.059(3) Uani 1 1 d . . . 
XPA1 O 0.3767(13) 0.8703(14) 0.5206(15) 0.090(5) Uani 1 1 d . . . 
XPA2 O 0.125(5) 0.136(3) 0.483(5) 0.034(11) Uani 0.24 1 d P . . 
W O 0.1178(16) 0.1003(11) 0.4416(16) 0.041(4) Uani 0.76 1 d P . . 
MH1A Nb 0.911(6) 0.264(6) 0.896(7) 0.0196(4) Uani 0.013(3) 1 d P . . 
MH1B Nb 0.9018(15) 0.1325(16) 0.7389(17) 0.0196(4) Uani 0.055(3) 1 d P . . 
MH2A Nb 0.3969(10) 0.1402(9) 0.7403(11) 0.0183(4) Uani 0.081(3) 1 d P . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
MH1 MH1B 0.76(2) . ? 
MH1 XM1 1.786(9) . ? 
MH1 MH1A 1.90(8) . ? 
MH1 O2 1.937(9) . ? 
MH1 O8 1.946(9) 1_655 ? 
MH1 O6 1.958(8) 1_655 ? 
MH1 O14 1.958(8) . ? 
MH1 XPM1 2.323(11) . ? 
MH1 MO3 3.5452(15) 1_556 ? 
MH1 AP2 3.58(5) 3_656 ? 
MH1 MO5 3.589(5) 4_656 ? 
MH1 AP1 3.708(7) 2_545 ? 
MH2 MH2A 0.828(12) . ? 
MH2 XM2 1.794(9) . ? 
MH2 O9 1.942(9) . ? 
MH2 O5 1.948(7) . ? 
MH2 O1 1.952(8) . ? 
MH2 O13 1.964(8) . ? 
MH2 XPM2 2.315(11) . ? 
MH2 AP2 3.45(5) 4_556 ? 
MH2 MO2 3.5409(15) 1_556 ? 
MH2 MO5 3.599(4) 1_556 ? 
MH2 AP1 3.660(7) 1_545 ? 
MH2 W 4.065(16) 4_556 ? 
MO1 XA1 1.853(9) 1_544 ? 
MO1 O10 1.907(9) . ? 
MO1 O12 1.927(9) 1_545 ? 
MO1 O3 2.026(8) 1_544 ? 
MO1 XA2 2.029(8) . ? 
MO1 O7 2.037(8) 1_554 ? 
MO1 MO4 3.209(3) 3 ? 
MO1 MO4 3.214(3) . ? 
MO1 MO5 3.244(5) 3_655 ? 
MO1 MO5 3.244(5) . ? 
MO1 MO3 3.566(2) 2_445 ? 
MO1 MO2 3.573(2) . ? 
MO2 XM2 2.296(9) 1_554 ? 
MO2 XM2 2.296(9) 4_556 ? 
MO2 O10 2.567(8) . ? 
MO2 O10 2.567(8) 4 ? 
MO2 O7 2.586(8) 1_554 ? 
MO2 O7 2.586(8) 4_556 ? 
MO2 MO5 3.194(4) 4 ? 
MO2 MO5 3.194(4) . ? 
MO2 MO4 3.2719(16) 4 ? 
MO2 MO4 3.2719(16) . ? 
MO2 Si2 3.498(3) 4_556 ? 
MO2 Si2 3.498(3) 1_554 ? 
MO3 MH1A 2.27(7) 1_554 ? 
MO3 MH1A 2.27(7) 4_656 ? 
MO3 XM1 2.294(9) 1_554 ? 
MO3 XM1 2.294(9) 4_656 ? 
MO3 O12 2.557(8) 3_665 ? 
MO3 O12 2.557(8) 2_545 ? 
MO3 O3 2.587(8) 3_666 ? 
MO3 O3 2.587(8) 2_544 ? 
MO3 MO5 3.193(4) . ? 
MO3 MO5 3.193(4) 4_655 ? 
MO3 MO4 3.2752(17) 1_655 ? 
MO3 MO4 3.2752(17) 4 ? 
MO4 O7 2.103(8) 1_554 ? 
MO4 O3 2.108(8) 3_566 ? 
MO4 XM2 2.135(9) 4_556 ? 
MO4 XM1 2.137(9) 1_454 ? 
MO4 XA2 2.215(8) . ? 
MO4 XA2 2.215(8) 3 ? 
MO4 MH1A 2.81(8) 1_454 ? 
MO4 MO1 3.209(3) 3 ? 
MO4 MO3 3.2752(17) 1_455 ? 
MO4 MO5 3.580(5) 4 ? 
MO5 MH1A 1.89(8) 4_656 ? 
MO5 O10 2.325(9) . ? 
MO5 O12 2.335(9) 3_665 ? 
MO5 XA1 2.429(9) 3_666 ? 
MO5 XA1 2.450(10) 1_544 ? 
MO5 XM2 2.458(11) 1_554 ? 
MO5 XM1 2.488(11) 4_656 ? 
MO5 MO1 3.244(5) 3_655 ? 
MO5 MH2A 3.278(13) 1_554 ? 
AP1 XPA1 2.145(19) . ? 
AP1 XA1 2.395(11) . ? 
AP1 O4 2.521(10) . ? 
AP1 O11 2.557(11) 3_666 ? 
AP1 O13 2.622(12) 1_565 ? 
AP1 O5 2.651(12) 1_565 ? 
AP1 O8 2.676(11) 2 ? 
AP1 O2 2.694(12) 2_455 ? 
AP1 MH2A 2.837(14) 1_565 ? 
AP1 Si2 3.153(7) 1_565 ? 
AP1 Si4 3.161(7) 3_676 ? 
AP1 Si1 3.166(7) . ? 
AP2 W 1.65(4) . ? 
AP2 XPA2 2.15(6) . ? 
AP2 XA2 2.46(4) . ? 
AP2 O9 2.49(5) 4_556 ? 
AP2 O1 2.51(4) 4_556 ? 
AP2 O6 2.59(5) 3_556 ? 
AP2 O14 2.61(4) 3_656 ? 
AP2 O11 2.83(3) . ? 
AP2 MH1B 2.83(5) 3_656 ? 
AP2 O4 2.88(3) 3_566 ? 
AP2 Si3 3.12(3) 4_556 ? 
AP2 Si1 3.17(3) 3_566 ? 
Si1 O1 1.593(8) 2_455 ? 
Si1 O2 1.615(9) 2_455 ? 
Si1 O3 1.623(9) . ? 
Si1 O4 1.635(8) . ? 
Si1 AP2 3.17(3) 3_566 ? 
Si1 MO3 3.513(3) 2_456 ? 
Si1 W 3.891(18) 3_566 ? 
Si2 O6 1.580(8) . ? 
Si2 O5 1.599(8) . ? 
Si2 O7 1.620(9) . ? 
Si2 O4 1.625(8) 1_545 ? 
Si2 MH1B 2.930(18) 1_455 ? 
Si2 MH2A 3.009(11) . ? 
Si2 AP1 3.153(7) 1_545 ? 
Si2 AP2 3.22(4) 3_556 ? 
Si2 MO2 3.498(3) 1_556 ? 
Si2 W 3.902(17) 3_556 ? 
Si2 W 4.147(18) . ? 
Si3 O8 1.599(9) . ? 
Si3 O9 1.600(9) . ? 
Si3 O10 1.618(10) 4_556 ? 
Si3 O11 1.631(8) 4_556 ? 
Si3 AP2 3.12(4) 4_556 ? 
Si3 AP1 3.185(7) 2_445 ? 
Si3 MO5 3.345(5) 4_556 ? 
Si3 W 3.907(19) 4_556 ? 
Si4 O13 1.585(8) 3_666 ? 
Si4 O14 1.595(9) 3_666 ? 
Si4 O12 1.611(9) . ? 
Si4 O11 1.620(9) 1_565 ? 
Si4 MH1B 3.005(17) 3_666 ? 
Si4 MH2A 3.023(11) 3_666 ? 
Si4 AP1 3.161(7) 3_676 ? 
Si4 AP2 3.18(3) 1_565 ? 
Si4 MO5 3.351(5) 3_665 ? 
Si4 W 3.919(19) 1_565 ? 
O1 Si1 1.593(8) 2_545 ? 
O1 AP2 2.51(4) 4_556 ? 
O1 W 3.086(19) 4_556 ? 
O2 Si1 1.615(9) 2_545 ? 
O2 MH1A 2.49(8) . ? 
O2 MH1B 2.55(2) . ? 
O2 AP1 2.694(12) 2_545 ? 
O3 MO1 2.026(8) 1_566 ? 
O3 MO4 2.108(8) 3_566 ? 
O3 MO3 2.587(8) 2_456 ? 
O4 Si2 1.625(8) 1_565 ? 
O4 AP2 2.88(3) 3_566 ? 
O4 W 3.352(19) 3_566 ? 
O5 MH2A 1.470(13) . ? 
O5 AP1 2.651(12) 1_545 ? 
O6 MH1B 1.491(19) 1_455 ? 
O6 MH1 1.958(8) 1_455 ? 
O6 AP2 2.59(5) 3_556 ? 
O6 W 3.093(19) 3_556 ? 
O6 W 3.59(2) . ? 
O7 MO1 2.037(8) 1_556 ? 
O7 MO4 2.103(8) 1_556 ? 
O7 MO2 2.586(8) 1_556 ? 
O8 MH1 1.946(9) 1_455 ? 
O8 MH1A 2.53(8) 1_455 ? 
O8 MH1B 2.53(2) 1_455 ? 
O8 AP1 2.676(11) 2_445 ? 
O9 AP2 2.49(5) 4_556 ? 
O9 MH2A 2.569(15) . ? 
O9 W 3.11(2) 4_556 ? 
O10 Si3 1.618(10) 4_556 ? 
O11 Si4 1.620(9) 1_545 ? 
O11 Si3 1.631(8) 4_556 ? 
O11 AP1 2.557(11) 3_666 ? 
O11 W 3.37(2) . ? 
O12 MO1 1.927(9) 1_565 ? 
O12 MO5 2.335(9) 3_665 ? 
O12 MO3 2.557(8) 2_455 ? 
O13 MH2A 1.494(13) . ? 
O13 Si4 1.585(8) 3_666 ? 
O13 AP1 2.622(11) 1_545 ? 
O14 MH1B 1.572(18) . ? 
O14 Si4 1.595(9) 3_666 ? 
O14 AP2 2.61(4) 3_656 ? 
O14 W 3.12(2) 3_656 ? 
XM1 MH1A 0.83(8) . ? 
XM1 MH1B 1.88(2) . ? 
XM1 MO4 2.137(9) 1_656 ? 
XM1 MO3 2.294(9) 1_556 ? 
XM1 MO5 2.488(11) 4_656 ? 
XM2 MH2A 2.064(16) . ? 
XM2 MO4 2.136(9) 4_556 ? 
XM2 MO2 2.296(9) 1_556 ? 
XM2 MO5 2.458(11) 1_556 ? 
XA1 MO1 1.852(9) 1_566 ? 
XA1 MO5 2.429(9) 3_666 ? 
XA1 MO5 2.450(10) 1_566 ? 
XA2 MO4 2.215(8) 3 ? 
XPM1 MH1B 2.47(2) . ? 
XPM1 XPA2 2.71(5) 1_655 ? 
XPM1 W 2.87(2) 1_655 ? 
XPM1 XPA1 2.881(19) 3_666 ? 
XPM1 XPA1 3.17(2) 2_545 ? 
XPM1 W 3.68(2) 3_656 ? 
XPM2 MH2A 2.379(17) . ? 
XPM2 XPA2 2.68(5) . ? 
XPM2 XPA1 2.881(19) 3_666 ? 
XPM2 W 2.88(2) . ? 
XPM2 XPA2 3.29(5) 4_556 ? 
XPM2 W 3.66(2) 4_556 ? 
XPA1 XPM2 2.881(19) 3_666 ? 
XPA1 XPM1 2.881(19) 3_666 ? 
XPA1 XPM1 3.17(2) 2_455 ? 
XPA2 W 0.61(4) . ? 
XPA2 XPM1 2.70(5) 1_455 ? 
XPA2 XPM2 3.29(5) 4_556 ? 
W XPM1 2.87(2) 1_455 ? 
W O1 3.086(19) 4_556 ? 
W O6 3.093(19) 3_556 ? 
W O9 3.11(2) 4_556 ? 
W O14 3.12(2) 3_656 ? 
W O4 3.352(19) 3_566 ? 
MH1A MO5 1.89(8) 4_656 ? 
MH1A MO3 2.27(7) 1_556 ? 
MH1A MH1B 2.28(8) . ? 
MH1A O8 2.53(8) 1_655 ? 
MH1A MO4 2.81(8) 1_656 ? 
MH1A MO2 3.77(7) 1_656 ? 
MH1B O6 1.491(19) 1_655 ? 
MH1B O8 2.53(2) 1_655 ? 
MH1B AP2 2.83(5) 3_656 ? 
MH1B Si2 2.930(18) 1_655 ? 
MH1B Si4 3.005(17) 3_666 ? 
MH1B W 3.45(3) 3_656 ? 
MH2A AP1 2.837(14) 1_545 ? 
MH2A Si4 3.023(11) 3_666 ? 
MH2A MO5 3.278(13) 1_556 ? 
MH2A MO2 3.621(12) 1_556 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
MH1B MH1 XM1 85.1(15) . . ? 
MH1B MH1 MH1A 111(3) . . ? 
XM1 MH1 MH1A 26(2) . . ? 
MH1B MH1 O2 136.9(12) . . ? 
XM1 MH1 O2 100.6(4) . . ? 
MH1A MH1 O2 81(2) . . ? 
MH1B MH1 O8 133.1(12) . 1_655 ? 
XM1 MH1 O8 99.5(4) . 1_655 ? 
MH1A MH1 O8 82(2) . 1_655 ? 
O2 MH1 O8 88.5(4) . 1_655 ? 
MH1B MH1 O6 42.7(12) . 1_655 ? 
XM1 MH1 O6 94.0(4) . 1_655 ? 
MH1A MH1 O6 113(2) . 1_655 ? 
O2 MH1 O6 165.4(4) . 1_655 ? 
O8 MH1 O6 90.4(4) 1_655 1_655 ? 
MH1B MH1 O14 49.3(12) . . ? 
XM1 MH1 O14 97.1(4) . . ? 
MH1A MH1 O14 113(2) . . ? 
O2 MH1 O14 87.6(4) . . ? 
O8 MH1 O14 163.5(4) 1_655 . ? 
O6 MH1 O14 89.3(4) 1_655 . ? 
MH1B MH1 XPM1 91.9(15) . . ? 
XM1 MH1 XPM1 175.6(4) . . ? 
MH1A MH1 XPM1 157(3) . . ? 
O2 MH1 XPM1 83.8(4) . . ? 
O8 MH1 XPM1 80.2(4) 1_655 . ? 
O6 MH1 XPM1 81.6(4) 1_655 . ? 
O14 MH1 XPM1 83.4(4) . . ? 
MH1B MH1 MO3 94.6(14) . 1_556 ? 
XM1 MH1 MO3 34.0(3) . 1_556 ? 
MH1A MH1 MO3 35(2) . 1_556 ? 
O2 MH1 MO3 71.4(3) . 1_556 ? 
O8 MH1 MO3 115.1(3) 1_655 1_556 ? 
O6 MH1 MO3 121.9(3) 1_655 1_556 ? 
O14 MH1 MO3 78.8(3) . 1_556 ? 
XPM1 MH1 MO3 149.9(3) . 1_556 ? 
MH1B MH1 AP2 6.2(15) . 3_656 ? 
XM1 MH1 AP2 90.6(7) . 3_656 ? 
MH1A MH1 AP2 116(3) . 3_656 ? 
O2 MH1 AP2 132.8(5) . 3_656 ? 
O8 MH1 AP2 134.9(5) 1_655 3_656 ? 
O6 MH1 AP2 44.9(5) 1_655 3_656 ? 
O14 MH1 AP2 45.3(5) . 3_656 ? 
XPM1 MH1 AP2 86.7(7) . 3_656 ? 
MO3 MH1 AP2 97.6(5) 1_556 3_656 ? 
MH1B MH1 MO5 121.6(15) . 4_656 ? 
XM1 MH1 MO5 39.6(3) . 4_656 ? 
MH1A MH1 MO5 19(2) . 4_656 ? 
O2 MH1 MO5 83.0(3) . 4_656 ? 
O8 MH1 MO5 63.7(3) 1_655 4_656 ? 
O6 MH1 MO5 109.5(3) 1_655 4_656 ? 
O14 MH1 MO5 131.5(3) . 4_656 ? 
XPM1 MH1 MO5 141.7(3) . 4_656 ? 
MO3 MH1 MO5 53.18(7) 1_556 4_656 ? 
AP2 MH1 MO5 127.6(6) 3_656 4_656 ? 
MH1B MH1 AP1 170.5(15) . 2_545 ? 
XM1 MH1 AP1 104.1(3) . 2_545 ? 
MH1A MH1 AP1 78(2) . 2_545 ? 
O2 MH1 AP1 44.5(3) . 2_545 ? 
O8 MH1 AP1 44.0(3) 1_655 2_545 ? 
O6 MH1 AP1 132.6(3) 1_655 2_545 ? 
O14 MH1 AP1 130.0(3) . 2_545 ? 
XPM1 MH1 AP1 78.7(3) . 2_545 ? 
MO3 MH1 AP1 94.40(11) 1_556 2_545 ? 
AP2 MH1 AP1 165.3(6) 3_656 2_545 ? 
MO5 MH1 AP1 66.80(13) 4_656 2_545 ? 
MH2A MH2 XM2 96.9(10) . . ? 
MH2A MH2 O9 131.8(8) . . ? 
XM2 MH2 O9 97.8(4) . . ? 
MH2A MH2 O5 44.0(8) . . ? 
XM2 MH2 O5 99.5(4) . . ? 
O9 MH2 O5 88.2(4) . . ? 
MH2A MH2 O1 133.8(8) . . ? 
XM2 MH2 O1 95.2(4) . . ? 
O9 MH2 O1 90.1(4) . . ? 
O5 MH2 O1 165.3(4) . . ? 
MH2A MH2 O13 44.8(8) . . ? 
XM2 MH2 O13 98.0(4) . . ? 
O9 MH2 O13 164.2(4) . . ? 
O5 MH2 O13 88.3(4) . . ? 
O1 MH2 O13 89.4(4) . . ? 
MH2A MH2 XPM2 84.2(10) . . ? 
XM2 MH2 XPM2 178.9(5) . . ? 
O9 MH2 XPM2 81.3(5) . . ? 
O5 MH2 XPM2 81.1(4) . . ? 
O1 MH2 XPM2 84.2(4) . . ? 
O13 MH2 XPM2 82.9(5) . . ? 
MH2A MH2 AP2 170.7(11) . 4_556 ? 
XM2 MH2 AP2 92.3(7) . 4_556 ? 
O9 MH2 AP2 45.1(5) . 4_556 ? 
O5 MH2 AP2 133.1(5) . 4_556 ? 
O1 MH2 AP2 45.8(5) . 4_556 ? 
O13 MH2 AP2 134.9(5) . 4_556 ? 
XPM2 MH2 AP2 86.6(7) . 4_556 ? 
MH2A MH2 MO2 88.9(9) . 1_556 ? 
XM2 MH2 MO2 34.4(3) . 1_556 ? 
O9 MH2 MO2 78.4(3) . 1_556 ? 
O5 MH2 MO2 70.8(3) . 1_556 ? 
O1 MH2 MO2 123.1(3) . 1_556 ? 
O13 MH2 MO2 114.8(3) . 1_556 ? 
XPM2 MH2 MO2 145.6(3) . 1_556 ? 
AP2 MH2 MO2 98.2(5) 4_556 1_556 ? 
MH2A MH2 MO5 61.0(9) . 1_556 ? 
XM2 MH2 MO5 38.3(3) . 1_556 ? 
O9 MH2 MO5 131.1(3) . 1_556 ? 
O5 MH2 MO5 82.3(3) . 1_556 ? 
O1 MH2 MO5 109.6(3) . 1_556 ? 
O13 MH2 MO5 63.5(3) . 1_556 ? 
XPM2 MH2 MO5 142.8(4) . 1_556 ? 
AP2 MH2 MO5 128.2(6) 4_556 1_556 ? 
MO2 MH2 MO5 53.14(7) 1_556 1_556 ? 
MH2A MH2 AP1 6.0(9) . 1_545 ? 
XM2 MH2 AP1 102.8(3) . 1_545 ? 
O9 MH2 AP1 130.6(3) . 1_545 ? 
O5 MH2 AP1 44.5(3) . 1_545 ? 
O1 MH2 AP1 131.3(3) . 1_545 ? 
O13 MH2 AP1 43.8(3) . 1_545 ? 
XPM2 MH2 AP1 78.3(4) . 1_545 ? 
AP2 MH2 AP1 164.9(6) 4_556 1_545 ? 
MO2 MH2 AP1 94.27(11) 1_556 1_545 ? 
MO5 MH2 AP1 66.56(13) 1_556 1_545 ? 
MH2A MH2 W 147.3(9) . 4_556 ? 
XM2 MH2 W 115.8(4) . 4_556 ? 
O9 MH2 W 47.7(4) . 4_556 ? 
O5 MH2 W 124.5(4) . 4_556 ? 
O1 MH2 W 47.0(3) . 4_556 ? 
O13 MH2 W 124.3(4) . 4_556 ? 
XPM2 MH2 W 63.1(4) . 4_556 ? 
AP2 MH2 W 23.5(6) 4_556 4_556 ? 
MO2 MH2 W 118.1(3) 1_556 4_556 ? 
MO5 MH2 W 149.9(3) 1_556 4_556 ? 
AP1 MH2 W 141.4(3) 1_545 4_556 ? 
XA1 MO1 O10 93.4(4) 1_544 . ? 
XA1 MO1 O12 93.2(4) 1_544 1_545 ? 
O10 MO1 O12 93.0(4) . 1_545 ? 
XA1 MO1 O3 92.7(4) 1_544 1_544 ? 
O10 MO1 O3 173.4(4) . 1_544 ? 
O12 MO1 O3 89.1(3) 1_545 1_544 ? 
XA1 MO1 XA2 173.9(4) 1_544 . ? 
O10 MO1 XA2 91.0(4) . . ? 
O12 MO1 XA2 90.7(4) 1_545 . ? 
O3 MO1 XA2 82.7(3) 1_544 . ? 
XA1 MO1 O7 93.5(4) 1_544 1_554 ? 
O10 MO1 O7 89.0(4) . 1_554 ? 
O12 MO1 O7 172.9(4) 1_545 1_554 ? 
O3 MO1 O7 88.2(3) 1_544 1_554 ? 
XA2 MO1 O7 82.4(3) . 1_554 ? 
XA1 MO1 MO4 132.6(3) 1_544 3 ? 
O10 MO1 MO4 134.0(3) . 3 ? 
O12 MO1 MO4 85.4(2) 1_545 3 ? 
O3 MO1 MO4 40.0(2) 1_544 3 ? 
XA2 MO1 MO4 43.1(2) . 3 ? 
O7 MO1 MO4 88.3(2) 1_554 3 ? 
XA1 MO1 MO4 133.3(3) 1_544 . ? 
O10 MO1 MO4 85.5(3) . . ? 
O12 MO1 MO4 133.5(3) 1_545 . ? 
O3 MO1 MO4 88.6(2) 1_544 . ? 
XA2 MO1 MO4 43.0(2) . . ? 
O7 MO1 MO4 39.8(2) 1_554 . ? 
MO4 MO1 MO4 64.20(6) 3 . ? 
XA1 MO1 MO5 47.9(3) 1_544 3_655 ? 
O10 MO1 MO5 96.9(3) . 3_655 ? 
O12 MO1 MO5 45.4(3) 1_545 3_655 ? 
O3 MO1 MO5 89.1(3) 1_544 3_655 ? 
XA2 MO1 MO5 135.6(2) . 3_655 ? 
O7 MO1 MO5 141.1(3) 1_554 3_655 ? 
MO4 MO1 MO5 113.22(10) 3 3_655 ? 
MO4 MO1 MO5 177.39(10) . 3_655 ? 
XA1 MO1 MO5 48.6(3) 1_544 . ? 
O10 MO1 MO5 45.0(3) . . ? 
O12 MO1 MO5 97.2(3) 1_545 . ? 
O3 MO1 MO5 140.9(3) 1_544 . ? 
XA2 MO1 MO5 135.4(3) . . ? 
O7 MO1 MO5 89.0(2) 1_554 . ? 
MO4 MO1 MO5 177.13(11) 3 . ? 
MO4 MO1 MO5 112.99(10) . . ? 
MO5 MO1 MO5 69.58(14) 3_655 . ? 
XA1 MO1 MO3 89.8(3) 1_544 2_445 ? 
O10 MO1 MO3 136.9(3) . 2_445 ? 
O12 MO1 MO3 44.0(2) 1_545 2_445 ? 
O3 MO1 MO3 45.5(2) 1_544 2_445 ? 
XA2 MO1 MO3 89.8(2) . 2_445 ? 
O7 MO1 MO3 133.7(2) 1_554 2_445 ? 
MO4 MO1 MO3 57.53(5) 3 2_445 ? 
MO4 MO1 MO3 121.73(7) . 2_445 ? 
MO5 MO1 MO3 55.69(8) 3_655 2_445 ? 
MO5 MO1 MO3 125.27(10) . 2_445 ? 
XA1 MO1 MO2 90.6(3) 1_544 . ? 
O10 MO1 MO2 43.9(3) . . ? 
O12 MO1 MO2 136.9(3) 1_545 . ? 
O3 MO1 MO2 133.5(2) 1_544 . ? 
XA2 MO1 MO2 89.7(2) . . ? 
O7 MO1 MO2 45.4(2) 1_554 . ? 
MO4 MO1 MO2 121.56(7) 3 . ? 
MO4 MO1 MO2 57.35(5) . . ? 
MO5 MO1 MO2 125.22(10) 3_655 . ? 
MO5 MO1 MO2 55.63(9) . . ? 
MO3 MO1 MO2 178.97(7) 2_445 . ? 
XM2 MO2 XM2 180.0 1_554 4_556 ? 
XM2 MO2 O10 95.8(3) 1_554 . ? 
XM2 MO2 O10 84.2(3) 4_556 . ? 
XM2 MO2 O10 84.2(3) 1_554 4 ? 
XM2 MO2 O10 95.8(3) 4_556 4 ? 
O10 MO2 O10 180.0 . 4 ? 
XM2 MO2 O7 100.1(3) 1_554 1_554 ? 
XM2 MO2 O7 79.9(3) 4_556 1_554 ? 
O10 MO2 O7 64.9(3) . 1_554 ? 
O10 MO2 O7 115.1(3) 4 1_554 ? 
XM2 MO2 O7 79.9(3) 1_554 4_556 ? 
XM2 MO2 O7 100.1(3) 4_556 4_556 ? 
O10 MO2 O7 115.1(3) . 4_556 ? 
O10 MO2 O7 64.9(3) 4 4_556 ? 
O7 MO2 O7 180.0(2) 1_554 4_556 ? 
XM2 MO2 MO5 130.0(3) 1_554 4 ? 
XM2 MO2 MO5 50.0(3) 4_556 4 ? 
O10 MO2 MO5 134.0(2) . 4 ? 
O10 MO2 MO5 46.0(2) 4 4 ? 
O7 MO2 MO5 98.51(19) 1_554 4 ? 
O7 MO2 MO5 81.49(19) 4_556 4 ? 
XM2 MO2 MO5 50.0(3) 1_554 . ? 
XM2 MO2 MO5 130.0(3) 4_556 . ? 
O10 MO2 MO5 46.0(2) . . ? 
O10 MO2 MO5 134.0(2) 4 . ? 
O7 MO2 MO5 81.49(19) 1_554 . ? 
O7 MO2 MO5 98.51(19) 4_556 . ? 
MO5 MO2 MO5 180.0 4 . ? 
XM2 MO2 MO4 40.5(2) 1_554 4 ? 
XM2 MO2 MO4 139.5(2) 4_556 4 ? 
O10 MO2 MO4 104.82(19) . 4 ? 
O10 MO2 MO4 75.18(19) 4 4 ? 
O7 MO2 MO4 140.03(18) 1_554 4 ? 
O7 MO2 MO4 39.98(18) 4_556 4 ? 
MO5 MO2 MO4 112.77(8) 4 4 ? 
MO5 MO2 MO4 67.23(8) . 4 ? 
XM2 MO2 MO4 139.5(2) 1_554 . ? 
XM2 MO2 MO4 40.5(2) 4_556 . ? 
O10 MO2 MO4 75.18(19) . . ? 
O10 MO2 MO4 104.82(19) 4 . ? 
O7 MO2 MO4 39.97(18) 1_554 . ? 
O7 MO2 MO4 140.02(18) 4_556 . ? 
MO5 MO2 MO4 67.23(8) 4 . ? 
MO5 MO2 MO4 112.77(8) . . ? 
MO4 MO2 MO4 180.0 4 . ? 
XM2 MO2 Si2 98.2(2) 1_554 4_556 ? 
XM2 MO2 Si2 81.8(2) 4_556 4_556 ? 
O10 MO2 Si2 95.4(2) . 4_556 ? 
O10 MO2 Si2 84.6(2) 4 4_556 ? 
O7 MO2 Si2 154.3(2) 1_554 4_556 ? 
O7 MO2 Si2 25.7(2) 4_556 4_556 ? 
MO5 MO2 Si2 83.17(9) 4 4_556 ? 
MO5 MO2 Si2 96.83(9) . 4_556 ? 
MO4 MO2 Si2 58.27(6) 4 4_556 ? 
MO4 MO2 Si2 121.73(6) . 4_556 ? 
XM2 MO2 Si2 81.8(2) 1_554 1_554 ? 
XM2 MO2 Si2 98.2(2) 4_556 1_554 ? 
O10 MO2 Si2 84.6(2) . 1_554 ? 
O10 MO2 Si2 95.4(2) 4 1_554 ? 
O7 MO2 Si2 25.7(2) 1_554 1_554 ? 
O7 MO2 Si2 154.3(2) 4_556 1_554 ? 
MO5 MO2 Si2 96.83(9) 4 1_554 ? 
MO5 MO2 Si2 83.17(9) . 1_554 ? 
MO4 MO2 Si2 121.72(6) 4 1_554 ? 
MO4 MO2 Si2 58.28(6) . 1_554 ? 
Si2 MO2 Si2 180.0 4_556 1_554 ? 
MH1A MO3 MH1A 179.999(4) 1_554 4_656 ? 
MH1A MO3 XM1 21(2) 1_554 1_554 ? 
MH1A MO3 XM1 159(2) 4_656 1_554 ? 
MH1A MO3 XM1 159(2) 1_554 4_656 ? 
MH1A MO3 XM1 21(2) 4_656 4_656 ? 
XM1 MO3 XM1 179.998(1) 1_554 4_656 ? 
MH1A MO3 O12 101(2) 1_554 3_665 ? 
MH1A MO3 O12 79(2) 4_656 3_665 ? 
XM1 MO3 O12 83.1(3) 1_554 3_665 ? 
XM1 MO3 O12 96.9(3) 4_656 3_665 ? 
MH1A MO3 O12 79(2) 1_554 2_545 ? 
MH1A MO3 O12 101(2) 4_656 2_545 ? 
XM1 MO3 O12 96.9(3) 1_554 2_545 ? 
XM1 MO3 O12 83.1(3) 4_656 2_545 ? 
O12 MO3 O12 180.00(19) 3_665 2_545 ? 
MH1A MO3 O3 98(2) 1_554 3_666 ? 
MH1A MO3 O3 82(2) 4_656 3_666 ? 
XM1 MO3 O3 79.8(3) 1_554 3_666 ? 
XM1 MO3 O3 100.2(3) 4_656 3_666 ? 
O12 MO3 O3 65.3(3) 3_665 3_666 ? 
O12 MO3 O3 114.7(3) 2_545 3_666 ? 
MH1A MO3 O3 82(2) 1_554 2_544 ? 
MH1A MO3 O3 98(2) 4_656 2_544 ? 
XM1 MO3 O3 100.2(3) 1_554 2_544 ? 
XM1 MO3 O3 79.8(3) 4_656 2_544 ? 
O12 MO3 O3 114.7(3) 3_665 2_544 ? 
O12 MO3 O3 65.3(3) 2_545 2_544 ? 
O3 MO3 O3 180.0 3_666 2_544 ? 
MH1A MO3 MO5 144(2) 1_554 . ? 
MH1A MO3 MO5 36(2) 4_656 . ? 
XM1 MO3 MO5 129.2(3) 1_554 . ? 
XM1 MO3 MO5 50.8(3) 4_656 . ? 
O12 MO3 MO5 46.3(2) 3_665 . ? 
O12 MO3 MO5 133.7(2) 2_545 . ? 
O3 MO3 MO5 81.36(19) 3_666 . ? 
O3 MO3 MO5 98.64(19) 2_544 . ? 
MH1A MO3 MO5 36(2) 1_554 4_655 ? 
MH1A MO3 MO5 144(2) 4_656 4_655 ? 
XM1 MO3 MO5 50.8(3) 1_554 4_655 ? 
XM1 MO3 MO5 129.2(3) 4_656 4_655 ? 
O12 MO3 MO5 133.7(2) 3_665 4_655 ? 
O12 MO3 MO5 46.3(2) 2_545 4_655 ? 
O3 MO3 MO5 98.63(19) 3_666 4_655 ? 
O3 MO3 MO5 81.37(19) 2_544 4_655 ? 
MO5 MO3 MO5 180.00(14) . 4_655 ? 
MH1A MO3 MO4 58(2) 1_554 1_655 ? 
MH1A MO3 MO4 122(2) 4_656 1_655 ? 
XM1 MO3 MO4 40.5(2) 1_554 1_655 ? 
XM1 MO3 MO4 139.5(2) 4_656 1_655 ? 
O12 MO3 MO4 75.34(19) 3_665 1_655 ? 
O12 MO3 MO4 104.66(19) 2_545 1_655 ? 
O3 MO3 MO4 40.02(18) 3_666 1_655 ? 
O3 MO3 MO4 139.98(18) 2_544 1_655 ? 
MO5 MO3 MO4 112.80(8) . 1_655 ? 
MO5 MO3 MO4 67.20(8) 4_655 1_655 ? 
MH1A MO3 MO4 122(2) 1_554 4 ? 
MH1A MO3 MO4 58(2) 4_656 4 ? 
XM1 MO3 MO4 139.5(2) 1_554 4 ? 
XM1 MO3 MO4 40.5(2) 4_656 4 ? 
O12 MO3 MO4 104.66(19) 3_665 4 ? 
O12 MO3 MO4 75.34(19) 2_545 4 ? 
O3 MO3 MO4 139.98(18) 3_666 4 ? 
O3 MO3 MO4 40.02(18) 2_544 4 ? 
MO5 MO3 MO4 67.20(8) . 4 ? 
MO5 MO3 MO4 112.80(8) 4_655 4 ? 
MO4 MO3 MO4 180.0 1_655 4 ? 
O7 MO4 O3 164.0(3) 1_554 3_566 ? 
O7 MO4 XM2 95.7(3) 1_554 4_556 ? 
O3 MO4 XM2 96.4(3) 3_566 4_556 ? 
O7 MO4 XM1 96.1(3) 1_554 1_454 ? 
O3 MO4 XM1 95.3(3) 3_566 1_454 ? 
XM2 MO4 XM1 85.1(4) 4_556 1_454 ? 
O7 MO4 XA2 76.6(3) 1_554 . ? 
O3 MO4 XA2 91.1(3) 3_566 . ? 
XM2 MO4 XA2 98.9(3) 4_556 . ? 
XM1 MO4 XA2 172.0(3) 1_454 . ? 
O7 MO4 XA2 90.9(3) 1_554 3 ? 
O3 MO4 XA2 76.5(3) 3_566 3 ? 
XM2 MO4 XA2 172.6(3) 4_556 3 ? 
XM1 MO4 XA2 97.7(3) 1_454 3 ? 
XA2 MO4 XA2 79.2(3) . 3 ? 
O7 MO4 MH1A 98.4(15) 1_554 1_454 ? 
O3 MO4 MH1A 95.1(14) 3_566 1_454 ? 
XM2 MO4 MH1A 73.7(16) 4_556 1_454 ? 
XM1 MO4 MH1A 11.5(16) 1_454 1_454 ? 
XA2 MO4 MH1A 170.8(14) . 1_454 ? 
XA2 MO4 MH1A 108.9(15) 3 1_454 ? 
O7 MO4 MO1 129.5(2) 1_554 3 ? 
O3 MO4 MO1 38.2(2) 3_566 3 ? 
XM2 MO4 MO1 134.4(2) 4_556 3 ? 
XM1 MO4 MO1 94.3(2) 1_454 3 ? 
XA2 MO4 MO1 87.9(2) . 3 ? 
XA2 MO4 MO1 38.7(2) 3 3 ? 
MH1A MO4 MO1 101.2(13) 1_454 3 ? 
O7 MO4 MO1 38.4(2) 1_554 . ? 
O3 MO4 MO1 129.7(2) 3_566 . ? 
XM2 MO4 MO1 95.2(3) 4_556 . ? 
XM1 MO4 MO1 134.4(2) 1_454 . ? 
XA2 MO4 MO1 38.6(2) . . ? 
XA2 MO4 MO1 87.7(2) 3 . ? 
MH1A MO4 MO1 135.1(14) 1_454 . ? 
MO1 MO4 MO1 115.80(6) 3 . ? 
O7 MO4 MO2 52.2(2) 1_554 . ? 
O3 MO4 MO2 140.7(2) 3_566 . ? 
XM2 MO4 MO2 44.3(2) 4_556 . ? 
XM1 MO4 MO2 83.3(2) 1_454 . ? 
XA2 MO4 MO2 94.7(2) . . ? 
XA2 MO4 MO2 142.7(2) 3 . ? 
MH1A MO4 MO2 76.2(13) 1_454 . ? 
MO1 MO4 MO2 177.33(6) 3 . ? 
MO1 MO4 MO2 66.84(5) . . ? 
O7 MO4 MO3 140.4(2) 1_554 1_455 ? 
O3 MO4 MO3 52.1(2) 3_566 1_455 ? 
XM2 MO4 MO3 82.7(2) 4_556 1_455 ? 
XM1 MO4 MO3 44.2(2) 1_454 1_455 ? 
XA2 MO4 MO3 142.9(2) . 1_455 ? 
XA2 MO4 MO3 94.5(2) 3 1_455 ? 
MH1A MO4 MO3 43.0(14) 1_454 1_455 ? 
MO1 MO4 MO3 66.71(5) 3 1_455 ? 
MO1 MO4 MO3 177.49(6) . 1_455 ? 
MO2 MO4 MO3 110.65(4) . 1_455 ? 
O7 MO4 MO5 98.0(2) 1_554 4 ? 
O3 MO4 MO5 98.0(2) 3_566 4 ? 
XM2 MO4 MO5 42.2(3) 4_556 4 ? 
XM1 MO4 MO5 43.0(3) 1_454 4 ? 
XA2 MO4 MO5 140.6(2) . 4 ? 
XA2 MO4 MO5 140.3(2) 3 4 ? 
MH1A MO4 MO5 31.6(16) 1_454 4 ? 
MO1 MO4 MO5 122.02(8) 3 4 ? 
MO1 MO4 MO5 122.19(8) . 4 ? 
MO2 MO4 MO5 55.35(7) . 4 ? 
MO3 MO4 MO5 55.31(7) 1_455 4 ? 
MH1A MO5 O10 101(2) 4_656 . ? 
MH1A MO5 O12 93(2) 4_656 3_665 ? 
O10 MO5 O12 157.2(4) . 3_665 ? 
MH1A MO5 XA1 89(2) 4_656 3_666 ? 
O10 MO5 XA1 92.3(3) . 3_666 ? 
O12 MO5 XA1 70.4(3) 3_665 3_666 ? 
MH1A MO5 XA1 166(2) 4_656 1_544 ? 
O10 MO5 XA1 69.9(3) . 1_544 ? 
O12 MO5 XA1 92.3(3) 3_665 1_544 ? 
XA1 MO5 XA1 81.3(3) 3_666 1_544 ? 
MH1A MO5 XM2 87(2) 4_656 1_554 ? 
O10 MO5 XM2 98.1(3) . 1_554 ? 
O12 MO5 XM2 100.2(3) 3_665 1_554 ? 
XA1 MO5 XM2 169.3(3) 3_666 1_554 ? 
XA1 MO5 XM2 104.7(3) 1_544 1_554 ? 
MH1A MO5 XM1 15(2) 4_656 4_656 ? 
O10 MO5 XM1 100.9(3) . 4_656 ? 
O12 MO5 XM1 97.8(3) 3_665 4_656 ? 
XA1 MO5 XM1 104.1(3) 3_666 4_656 ? 
XA1 MO5 XM1 169.7(3) 1_544 4_656 ? 
XM2 MO5 XM1 71.5(3) 1_554 4_656 ? 
MH1A MO5 MO3 44(2) 4_656 . ? 
O10 MO5 MO3 145.6(3) . . ? 
O12 MO5 MO3 52.3(2) 3_665 . ? 
XA1 MO5 MO3 90.0(2) 3_666 . ? 
XA1 MO5 MO3 144.2(2) 1_544 . ? 
XM2 MO5 MO3 80.0(2) 1_554 . ? 
XM1 MO5 MO3 45.6(2) 4_656 . ? 
MH1A MO5 MO2 92(2) 4_656 . ? 
O10 MO5 MO2 52.6(2) . . ? 
O12 MO5 MO2 145.0(3) 3_665 . ? 
XA1 MO5 MO2 144.3(2) 3_666 . ? 
XA1 MO5 MO2 90.5(2) 1_544 . ? 
XM2 MO5 MO2 45.7(2) 1_554 . ? 
XM1 MO5 MO2 80.0(2) 4_656 . ? 
MO3 MO5 MO2 114.91(14) . . ? 
MH1A MO5 MO1 90(2) 4_656 3_655 ? 
O10 MO5 MO1 125.8(3) . 3_655 ? 
O12 MO5 MO1 36.0(2) 3_665 3_655 ? 
XA1 MO5 MO1 34.5(2) 3_666 3_655 ? 
XA1 MO5 MO1 87.4(2) 1_544 3_655 ? 
XM2 MO5 MO1 135.7(3) 1_554 3_655 ? 
XM1 MO5 MO1 102.0(2) 4_656 3_655 ? 
MO3 MO5 MO1 67.27(8) . 3_655 ? 
MO2 MO5 MO1 177.81(16) . 3_655 ? 
MH1A MO5 MO1 136(2) 4_656 . ? 
O10 MO5 MO1 35.4(2) . . ? 
O12 MO5 MO1 126.0(3) 3_665 . ? 
XA1 MO5 MO1 87.8(2) 3_666 . ? 
XA1 MO5 MO1 34.5(2) 1_544 . ? 
XM2 MO5 MO1 102.2(2) 1_554 . ? 
XM1 MO5 MO1 135.9(2) 4_656 . ? 
MO3 MO5 MO1 177.67(16) . . ? 
MO2 MO5 MO1 67.40(8) . . ? 
MO1 MO5 MO1 110.42(14) 3_655 . ? 
MH1A MO5 MH2A 121(3) 4_656 1_554 ? 
O10 MO5 MH2A 107.2(3) . 1_554 ? 
O12 MO5 MH2A 79.6(3) 3_665 1_554 ? 
XA1 MO5 MH2A 139.2(3) 3_666 1_554 ? 
XA1 MO5 MH2A 72.9(3) 1_544 1_554 ? 
XM2 MO5 MH2A 39.0(3) 1_554 1_554 ? 
XM1 MO5 MH2A 106.8(3) 4_656 1_554 ? 
MO3 MO5 MH2A 92.9(2) . 1_554 ? 
MO2 MO5 MH2A 68.0(2) . 1_554 ? 
MO1 MO5 MH2A 112.0(2) 3_655 1_554 ? 
MO1 MO5 MH2A 88.3(2) . 1_554 ? 
XPA1 AP1 XA1 167.3(6) . . ? 
XPA1 AP1 O4 93.5(5) . . ? 
XA1 AP1 O4 79.0(3) . . ? 
XPA1 AP1 O11 91.2(5) . 3_666 ? 
XA1 AP1 O11 96.1(4) . 3_666 ? 
O4 AP1 O11 175.0(4) . 3_666 ? 
XPA1 AP1 O13 103.5(6) . 1_565 ? 
XA1 AP1 O13 89.2(4) . 1_565 ? 
O4 AP1 O13 121.4(4) . 1_565 ? 
O11 AP1 O13 58.7(3) 3_666 1_565 ? 
XPA1 AP1 O5 104.7(6) . 1_565 ? 
XA1 AP1 O5 80.4(4) . 1_565 ? 
O4 AP1 O5 59.3(3) . 1_565 ? 
O11 AP1 O5 120.9(4) 3_666 1_565 ? 
O13 AP1 O5 62.2(3) 1_565 1_565 ? 
XPA1 AP1 O8 87.8(6) . 2 ? 
XA1 AP1 O8 87.2(4) . 2 ? 
O4 AP1 O8 120.0(4) . 2 ? 
O11 AP1 O8 58.6(3) 3_666 2 ? 
O13 AP1 O8 116.4(3) 1_565 2 ? 
O5 AP1 O8 167.4(4) 1_565 2 ? 
XPA1 AP1 O2 88.4(5) . 2_455 ? 
XA1 AP1 O2 78.9(4) . 2_455 ? 
O4 AP1 O2 59.4(3) . 2_455 ? 
O11 AP1 O2 119.2(4) 3_666 2_455 ? 
O13 AP1 O2 167.8(4) 1_565 2_455 ? 
O5 AP1 O2 117.8(3) 1_565 2_455 ? 
O8 AP1 O2 60.6(3) 2 2_455 ? 
XPA1 AP1 MH2A 107.9(6) . 1_565 ? 
XA1 AP1 MH2A 82.5(4) . 1_565 ? 
O4 AP1 MH2A 90.0(3) . 1_565 ? 
O11 AP1 MH2A 90.0(3) 3_666 1_565 ? 
O13 AP1 MH2A 31.5(3) 1_565 1_565 ? 
O5 AP1 MH2A 30.8(3) 1_565 1_565 ? 
O8 AP1 MH2A 145.8(4) 2 1_565 ? 
O2 AP1 MH2A 146.6(4) 2_455 1_565 ? 
XPA1 AP1 Si2 108.4(5) . 1_565 ? 
XA1 AP1 Si2 70.0(3) . 1_565 ? 
O4 AP1 Si2 30.81(19) . 1_565 ? 
O11 AP1 Si2 147.7(3) 3_666 1_565 ? 
O13 AP1 Si2 91.3(3) 1_565 1_565 ? 
O5 AP1 Si2 30.44(18) 1_565 1_565 ? 
O8 AP1 Si2 144.2(3) 2 1_565 ? 
O2 AP1 Si2 87.5(2) 2_455 1_565 ? 
MH2A AP1 Si2 60.0(3) 1_565 1_565 ? 
XPA1 AP1 Si4 106.3(4) . 3_676 ? 
XA1 AP1 Si4 85.1(3) . 3_676 ? 
O4 AP1 Si4 147.9(3) . 3_676 ? 
O11 AP1 Si4 30.7(2) 3_666 3_676 ? 
O13 AP1 Si4 30.00(18) 1_565 3_676 ? 
O5 AP1 Si4 90.8(3) 1_565 3_676 ? 
O8 AP1 Si4 86.5(3) 2 3_676 ? 
O2 AP1 Si4 143.7(3) 2_455 3_676 ? 
MH2A AP1 Si4 60.2(3) 1_565 3_676 ? 
Si2 AP1 Si4 117.2(2) 1_565 3_676 ? 
XPA1 AP1 Si1 99.3(4) . . ? 
XA1 AP1 Si1 69.0(3) . . ? 
O4 AP1 Si1 30.84(19) . . ? 
O11 AP1 Si1 146.4(3) 3_666 . ? 
O13 AP1 Si1 145.5(3) 1_565 . ? 
O5 AP1 Si1 87.2(2) 1_565 . ? 
O8 AP1 Si1 89.8(3) 2 . ? 
O2 AP1 Si1 30.7(2) 2_455 . ? 
MH2A AP1 Si1 116.2(3) 1_565 . ? 
Si2 AP1 Si1 56.83(12) 1_565 . ? 
Si4 AP1 Si1 153.9(3) 3_676 . ? 
W AP2 XPA2 10.4(16) . . ? 
W AP2 XA2 177(3) . . ? 
XPA2 AP2 XA2 172(3) . . ? 
W AP2 O9 95.3(19) . 4_556 ? 
XPA2 AP2 O9 85.9(19) . 4_556 ? 
XA2 AP2 O9 86.7(13) . 4_556 ? 
W AP2 O1 93.4(17) . 4_556 ? 
XPA2 AP2 O1 86(2) . 4_556 ? 
XA2 AP2 O1 89.7(13) . 4_556 ? 
O9 AP2 O1 66.8(13) 4_556 4_556 ? 
W AP2 O6 91.0(19) . 3_556 ? 
XPA2 AP2 O6 100(2) . 3_556 ? 
XA2 AP2 O6 87.1(13) . 3_556 ? 
O9 AP2 O6 173.8(16) 4_556 3_556 ? 
O1 AP2 O6 113.1(10) 4_556 3_556 ? 
W AP2 O14 91.6(19) . 3_656 ? 
XPA2 AP2 O14 100(2) . 3_656 ? 
XA2 AP2 O14 85.2(12) . 3_656 ? 
O9 AP2 O14 115.6(10) 4_556 3_656 ? 
O1 AP2 O14 174.2(16) 4_556 3_656 ? 
O6 AP2 O14 63.9(12) 3_556 3_656 ? 
W AP2 O11 94.3(14) . . ? 
XPA2 AP2 O11 93.2(17) . . ? 
XA2 AP2 O11 84.5(9) . . ? 
O9 AP2 O11 58.6(7) 4_556 . ? 
O1 AP2 O11 125.3(18) 4_556 . ? 
O6 AP2 O11 120.8(16) 3_556 . ? 
O14 AP2 O11 57.0(6) 3_656 . ? 
W AP2 MH1B 97(2) . 3_656 ? 
XPA2 AP2 MH1B 108(2) . 3_656 ? 
XA2 AP2 MH1B 79.5(12) . 3_656 ? 
O9 AP2 MH1B 146.4(12) 4_556 3_656 ? 
O1 AP2 MH1B 142.7(13) 4_556 3_656 ? 
O6 AP2 MH1B 31.6(7) 3_556 3_656 ? 
O14 AP2 MH1B 33.3(7) 3_656 3_656 ? 
O11 AP2 MH1B 89.4(11) . 3_656 ? 
W AP2 O4 91.4(13) . 3_566 ? 
XPA2 AP2 O4 92.9(16) . 3_566 ? 
XA2 AP2 O4 89.7(10) . 3_566 ? 
O9 AP2 O4 123.9(16) 4_556 3_566 ? 
O1 AP2 O4 57.3(6) 4_556 3_566 ? 
O6 AP2 O4 55.9(7) 3_556 3_566 ? 
O14 AP2 O4 119.8(17) 3_656 3_566 ? 
O11 AP2 O4 173.5(15) . 3_566 ? 
MH1B AP2 O4 86.8(12) 3_656 3_566 ? 
W AP2 Si3 106.1(16) . 4_556 ? 
XPA2 AP2 Si3 100.0(18) . 4_556 ? 
XA2 AP2 Si3 74.3(9) . 4_556 ? 
O9 AP2 Si3 30.7(4) 4_556 4_556 ? 
O1 AP2 Si3 95.0(15) 4_556 4_556 ? 
O6 AP2 Si3 146.3(14) 3_556 4_556 ? 
O14 AP2 Si3 86.3(7) 3_656 4_556 ? 
O11 AP2 Si3 31.4(4) . 4_556 ? 
MH1B AP2 Si3 115.7(11) 3_656 4_556 ? 
O4 AP2 Si3 148.5(17) 3_566 4_556 ? 
W AP2 Si1 103.2(14) . 3_566 ? 
XPA2 AP2 Si1 99.4(18) . 3_566 ? 
XA2 AP2 Si1 79.2(9) . 3_566 ? 
O9 AP2 Si1 94.1(14) 4_556 3_566 ? 
O1 AP2 Si1 29.8(4) 4_556 3_566 ? 
O6 AP2 Si1 84.7(8) 3_556 3_566 ? 
O14 AP2 Si1 145.6(15) 3_656 3_566 ? 
O11 AP2 Si1 149.1(17) . 3_566 ? 
MH1B AP2 Si1 112.9(12) 3_656 3_566 ? 
O4 AP2 Si1 30.9(3) 3_566 3_566 ? 
Si3 AP2 Si1 118.0(15) 4_556 3_566 ? 
O1 Si1 O2 111.7(5) 2_455 2_455 ? 
O1 Si1 O3 111.5(5) 2_455 . ? 
O2 Si1 O3 110.8(5) 2_455 . ? 
O1 Si1 O4 107.6(5) 2_455 . ? 
O2 Si1 O4 105.6(5) 2_455 . ? 
O3 Si1 O4 109.3(4) . . ? 
O1 Si1 AP1 142.8(4) 2_455 . ? 
O2 Si1 AP1 58.3(4) 2_455 . ? 
O3 Si1 AP1 105.1(3) . . ? 
O4 Si1 AP1 52.2(3) . . ? 
O1 Si1 AP2 51.7(9) 2_455 3_566 ? 
O2 Si1 AP2 149.5(8) 2_455 3_566 ? 
O3 Si1 AP2 99.6(7) . 3_566 ? 
O4 Si1 AP2 64.7(9) . 3_566 ? 
AP1 Si1 AP2 116.7(8) . 3_566 ? 
O1 Si1 MO3 105.1(3) 2_455 2_456 ? 
O2 Si1 MO3 74.7(4) 2_455 2_456 ? 
O3 Si1 MO3 43.4(3) . 2_456 ? 
O4 Si1 MO3 144.2(3) . 2_456 ? 
AP1 Si1 MO3 105.59(15) . 2_456 ? 
AP2 Si1 MO3 130.9(7) 3_566 2_456 ? 
O1 Si1 W 48.8(4) 2_455 3_566 ? 
O2 Si1 W 125.3(5) 2_455 3_566 ? 
O3 Si1 W 123.8(4) . 3_566 ? 
O4 Si1 W 58.9(4) . 3_566 ? 
AP1 Si1 W 104.5(3) . 3_566 ? 
AP2 Si1 W 24.3(7) 3_566 3_566 ? 
MO3 Si1 W 149.7(3) 2_456 3_566 ? 
O6 Si2 O5 113.4(5) . . ? 
O6 Si2 O7 111.3(5) . . ? 
O5 Si2 O7 110.7(5) . . ? 
O6 Si2 O4 107.1(5) . 1_545 ? 
O5 Si2 O4 105.1(5) . 1_545 ? 
O7 Si2 O4 109.0(4) . 1_545 ? 
O6 Si2 MH1B 16.9(5) . 1_455 ? 
O5 Si2 MH1B 121.1(6) . 1_455 ? 
O7 Si2 MH1B 94.5(5) . 1_455 ? 
O4 Si2 MH1B 115.7(5) 1_545 1_455 ? 
O6 Si2 MH2A 122.2(5) . . ? 
O5 Si2 MH2A 10.8(4) . . ? 
O7 Si2 MH2A 100.6(4) . . ? 
O4 Si2 MH2A 106.0(4) 1_545 . ? 
MH1B Si2 MH2A 127.7(5) 1_455 . ? 
O6 Si2 AP1 143.0(4) . 1_545 ? 
O5 Si2 AP1 57.2(4) . 1_545 ? 
O7 Si2 AP1 105.0(3) . 1_545 ? 
O4 Si2 AP1 52.6(3) 1_545 1_545 ? 
MH1B Si2 AP1 159.7(4) 1_455 1_545 ? 
MH2A Si2 AP1 54.8(3) . 1_545 ? 
O6 Si2 AP2 52.7(9) . 3_556 ? 
O5 Si2 AP2 150.3(8) . 3_556 ? 
O7 Si2 AP2 99.0(7) . 3_556 ? 
O4 Si2 AP2 63.1(8) 1_545 3_556 ? 
MH1B Si2 AP2 54.4(9) 1_455 3_556 ? 
MH2A Si2 AP2 159.9(7) . 3_556 ? 
AP1 Si2 AP2 115.5(7) 1_545 3_556 ? 
O6 Si2 MO2 105.9(4) . 1_556 ? 
O5 Si2 MO2 74.4(4) . 1_556 ? 
O7 Si2 MO2 43.9(3) . 1_556 ? 
O4 Si2 MO2 143.9(3) 1_545 1_556 ? 
MH1B Si2 MO2 93.0(4) 1_455 1_556 ? 
MH2A Si2 MO2 67.1(3) . 1_556 ? 
AP1 Si2 MO2 104.95(15) 1_545 1_556 ? 
AP2 Si2 MO2 132.0(6) 3_556 1_556 ? 
O6 Si2 W 48.6(4) . 3_556 ? 
O5 Si2 W 125.8(5) . 3_556 ? 
O7 Si2 W 123.4(4) . 3_556 ? 
O4 Si2 W 58.5(4) 1_545 3_556 ? 
MH1B Si2 W 58.6(5) 1_455 3_556 ? 
MH2A Si2 W 135.7(4) . 3_556 ? 
AP1 Si2 W 104.6(3) 1_545 3_556 ? 
AP2 Si2 W 24.4(7) 3_556 3_556 ? 
MO2 Si2 W 150.3(3) 1_556 3_556 ? 
O6 Si2 W 58.8(5) . . ? 
O5 Si2 W 63.2(4) . . ? 
O7 Si2 W 158.8(4) . . ? 
O4 Si2 W 92.2(4) 1_545 . ? 
MH1B Si2 W 74.3(5) 1_455 . ? 
MH2A Si2 W 74.0(3) . . ? 
AP1 Si2 W 88.8(3) 1_545 . ? 
AP2 Si2 W 89.1(7) 3_556 . ? 
MO2 Si2 W 117.5(2) 1_556 . ? 
W Si2 W 66.3(4) 3_556 . ? 
O8 Si3 O9 113.1(5) . . ? 
O8 Si3 O10 110.2(5) . 4_556 ? 
O9 Si3 O10 111.1(5) . 4_556 ? 
O8 Si3 O11 105.1(5) . 4_556 ? 
O9 Si3 O11 108.4(5) . 4_556 ? 
O10 Si3 O11 108.8(5) 4_556 4_556 ? 
O8 Si3 AP2 150.9(8) . 4_556 ? 
O9 Si3 AP2 52.6(9) . 4_556 ? 
O10 Si3 AP2 98.9(7) 4_556 4_556 ? 
O11 Si3 AP2 64.4(9) 4_556 4_556 ? 
O8 Si3 AP1 57.1(4) . 2_445 ? 
O9 Si3 AP1 144.5(4) . 2_445 ? 
O10 Si3 AP1 103.9(3) 4_556 2_445 ? 
O11 Si3 AP1 52.9(3) 4_556 2_445 ? 
AP2 Si3 AP1 117.2(8) 4_556 2_445 ? 
O8 Si3 MO5 72.3(4) . 4_556 ? 
O9 Si3 MO5 137.1(4) . 4_556 ? 
O10 Si3 MO5 39.1(3) 4_556 4_556 ? 
O11 Si3 MO5 110.9(4) 4_556 4_556 ? 
AP2 Si3 MO5 136.5(7) 4_556 4_556 ? 
AP1 Si3 MO5 75.91(15) 2_445 4_556 ? 
O8 Si3 W 127.0(5) . 4_556 ? 
O9 Si3 W 49.3(4) . 4_556 ? 
O10 Si3 W 122.8(4) 4_556 4_556 ? 
O11 Si3 W 59.1(4) 4_556 4_556 ? 
AP2 Si3 W 23.9(7) 4_556 4_556 ? 
AP1 Si3 W 106.1(3) 2_445 4_556 ? 
MO5 Si3 W 158.9(3) 4_556 4_556 ? 
O13 Si4 O14 113.5(6) 3_666 3_666 ? 
O13 Si4 O12 110.3(5) 3_666 . ? 
O14 Si4 O12 111.8(5) 3_666 . ? 
O13 Si4 O11 104.8(5) 3_666 1_565 ? 
O14 Si4 O11 107.8(5) 3_666 1_565 ? 
O12 Si4 O11 108.1(5) . 1_565 ? 
O13 Si4 MH1B 123.7(6) 3_666 3_666 ? 
O14 Si4 MH1B 18.3(5) 3_666 3_666 ? 
O12 Si4 MH1B 93.6(5) . 3_666 ? 
O11 Si4 MH1B 115.1(5) 1_565 3_666 ? 
O13 Si4 MH2A 10.6(5) 3_666 3_666 ? 
O14 Si4 MH2A 121.5(5) 3_666 3_666 ? 
O12 Si4 MH2A 100.0(4) . 3_666 ? 
O11 Si4 MH2A 106.8(4) 1_565 3_666 ? 
MH1B Si4 MH2A 128.9(5) 3_666 3_666 ? 
O13 Si4 AP1 55.8(4) 3_666 3_676 ? 
O14 Si4 AP1 143.9(4) 3_666 3_676 ? 
O12 Si4 AP1 103.8(3) . 3_676 ? 
O11 Si4 AP1 53.6(3) 1_565 3_676 ? 
MH1B Si4 AP1 161.5(4) 3_666 3_676 ? 
MH2A Si4 AP1 54.6(3) 3_666 3_676 ? 
O13 Si4 AP2 151.6(8) 3_666 1_565 ? 
O14 Si4 AP2 54.6(9) 3_666 1_565 ? 
O12 Si4 AP2 98.0(7) . 1_565 ? 
O11 Si4 AP2 62.4(9) 1_565 1_565 ? 
MH1B Si4 AP2 54.2(9) 3_666 1_565 ? 
MH2A Si4 AP2 161.3(7) 3_666 1_565 ? 
AP1 Si4 AP2 115.9(8) 3_676 1_565 ? 
O13 Si4 MO5 72.2(4) 3_666 3_665 ? 
O14 Si4 MO5 138.2(4) 3_666 3_665 ? 
O12 Si4 MO5 39.2(3) . 3_665 ? 
O11 Si4 MO5 110.3(4) 1_565 3_665 ? 
MH1B Si4 MO5 123.0(4) 3_666 3_665 ? 
MH2A Si4 MO5 61.6(3) 3_666 3_665 ? 
AP1 Si4 MO5 75.36(16) 3_676 3_665 ? 
AP2 Si4 MO5 135.1(7) 1_565 3_665 ? 
O13 Si4 W 127.6(5) 3_666 1_565 ? 
O14 Si4 W 49.3(4) 3_666 1_565 ? 
O12 Si4 W 122.1(4) . 1_565 ? 
O11 Si4 W 58.7(4) 1_565 1_565 ? 
MH1B Si4 W 58.0(5) 3_666 1_565 ? 
MH2A Si4 W 137.7(4) 3_666 1_565 ? 
AP1 Si4 W 106.3(3) 3_676 1_565 ? 
AP2 Si4 W 24.1(7) 1_565 1_565 ? 
MO5 Si4 W 157.8(3) 3_665 1_565 ? 
Si1 O1 MH2 141.8(6) 2_545 . ? 
Si1 O1 AP2 98.5(9) 2_545 4_556 ? 
MH2 O1 AP2 100.4(9) . 4_556 ? 
Si1 O1 W 108.3(5) 2_545 4_556 ? 
MH2 O1 W 105.4(4) . 4_556 ? 
AP2 O1 W 32.2(9) 4_556 4_556 ? 
Si1 O2 MH1 154.6(7) 2_545 . ? 
Si1 O2 MH1A 111.7(18) 2_545 . ? 
MH1 O2 MH1A 48.8(19) . . ? 
Si1 O2 MH1B 148.0(7) 2_545 . ? 
MH1 O2 MH1B 11.8(4) . . ? 
MH1A O2 MH1B 53.9(19) . . ? 
Si1 O2 AP1 91.1(4) 2_545 2_545 ? 
MH1 O2 AP1 105.2(4) . 2_545 ? 
MH1A O2 AP1 94.4(18) . 2_545 ? 
MH1B O2 AP1 116.7(5) . 2_545 ? 
Si1 O3 MO1 123.5(4) . 1_566 ? 
Si1 O3 MO4 124.2(4) . 3_566 ? 
MO1 O3 MO4 101.8(4) 1_566 3_566 ? 
Si1 O3 MO3 111.0(4) . 2_456 ? 
MO1 O3 MO3 100.5(3) 1_566 2_456 ? 
MO4 O3 MO3 87.9(3) 3_566 2_456 ? 
Si2 O4 Si1 134.5(6) 1_565 . ? 
Si2 O4 AP1 96.6(4) 1_565 . ? 
Si1 O4 AP1 96.9(4) . . ? 
Si2 O4 AP2 86.7(10) 1_565 3_566 ? 
Si1 O4 AP2 84.4(10) . 3_566 ? 
AP1 O4 AP2 173.8(8) . 3_566 ? 
Si2 O4 W 97.1(5) 1_565 3_566 ? 
Si1 O4 W 96.5(4) . 3_566 ? 
AP1 O4 W 144.5(5) . 3_566 ? 
AP2 O4 W 29.4(8) 3_566 3_566 ? 
MH2A O5 Si2 157.5(9) . . ? 
MH2A O5 MH2 23.1(5) . . ? 
Si2 O5 MH2 155.1(7) . . ? 
MH2A O5 AP1 81.6(6) . 1_545 ? 
Si2 O5 AP1 92.4(4) . 1_545 ? 
MH2 O5 AP1 104.4(4) . 1_545 ? 
MH1B O6 Si2 145.2(11) 1_455 . ? 
MH1B O6 MH1 20.2(8) 1_455 1_455 ? 
Si2 O6 MH1 141.6(6) . 1_455 ? 
MH1B O6 AP2 82.9(11) 1_455 3_556 ? 
Si2 O6 AP2 98.4(9) . 3_556 ? 
MH1 O6 AP2 102.9(8) 1_455 3_556 ? 
MH1B O6 W 90.7(9) 1_455 3_556 ? 
Si2 O6 W 108.8(5) . 3_556 ? 
MH1 O6 W 106.2(5) 1_455 3_556 ? 
AP2 O6 W 32.1(9) 3_556 3_556 ? 
MH1B O6 W 112.3(9) 1_455 . ? 
Si2 O6 W 99.1(5) . . ? 
MH1 O6 W 100.9(4) 1_455 . ? 
AP2 O6 W 113.9(9) 3_556 . ? 
W O6 W 82.1(5) 3_556 . ? 
Si2 O7 MO1 123.8(5) . 1_556 ? 
Si2 O7 MO4 124.4(4) . 1_556 ? 
MO1 O7 MO4 101.8(4) 1_556 1_556 ? 
Si2 O7 MO2 110.4(4) . 1_556 ? 
MO1 O7 MO2 100.5(3) 1_556 1_556 ? 
MO4 O7 MO2 87.9(3) 1_556 1_556 ? 
Si3 O8 MH1 153.9(6) . 1_455 ? 
Si3 O8 MH1A 113.6(17) . 1_455 ? 
MH1 O8 MH1A 48.0(18) 1_455 1_455 ? 
Si3 O8 MH1B 145.8(7) . 1_455 ? 
MH1 O8 MH1B 12.7(4) 1_455 1_455 ? 
MH1A O8 MH1B 53.7(19) 1_455 1_455 ? 
Si3 O8 AP1 92.8(4) . 2_445 ? 
MH1 O8 AP1 105.6(4) 1_455 2_445 ? 
MH1A O8 AP1 94.0(18) 1_455 2_445 ? 
MH1B O8 AP1 118.0(5) 1_455 2_445 ? 
Si3 O9 MH2 142.7(7) . . ? 
Si3 O9 AP2 96.7(9) . 4_556 ? 
MH2 O9 AP2 101.4(8) . 4_556 ? 
Si3 O9 MH2A 137.2(6) . . ? 
MH2 O9 MH2A 13.9(3) . . ? 
AP2 O9 MH2A 115.0(9) 4_556 . ? 
Si3 O9 W 107.7(6) . 4_556 ? 
MH2 O9 W 104.8(5) . 4_556 ? 
AP2 O9 W 31.8(9) 4_556 4_556 ? 
MH2A O9 W 114.4(5) . 4_556 ? 
Si3 O10 MO1 130.7(5) 4_556 . ? 
Si3 O10 MO5 114.9(4) 4_556 . ? 
MO1 O10 MO5 99.6(4) . . ? 
Si3 O10 MO2 113.7(4) 4_556 . ? 
MO1 O10 MO2 105.0(4) . . ? 
MO5 O10 MO2 81.4(3) . . ? 
Si4 O11 Si3 134.5(6) 1_545 4_556 ? 
Si4 O11 AP1 95.7(4) 1_545 3_666 ? 
Si3 O11 AP1 96.5(4) 4_556 3_666 ? 
Si4 O11 AP2 87.0(10) 1_545 . ? 
Si3 O11 AP2 84.2(10) 4_556 . ? 
AP1 O11 AP2 175.3(8) 3_666 . ? 
Si4 O11 W 97.1(5) 1_545 . ? 
Si3 O11 W 96.3(5) 4_556 . ? 
AP1 O11 W 146.4(5) 3_666 . ? 
AP2 O11 W 29.1(8) . . ? 
Si4 O12 MO1 131.4(5) . 1_565 ? 
Si4 O12 MO5 115.0(5) . 3_665 ? 
MO1 O12 MO5 98.7(4) 1_565 3_665 ? 
Si4 O12 MO3 113.9(4) . 2_455 ? 
MO1 O12 MO3 104.5(4) 1_565 2_455 ? 
MO5 O12 MO3 81.4(3) 3_665 2_455 ? 
MH2A O13 Si4 158.2(9) . 3_666 ? 
MH2A O13 MH2 23.0(5) . . ? 
Si4 O13 MH2 153.6(6) 3_666 . ? 
MH2A O13 AP1 82.2(6) . 1_545 ? 
Si4 O13 AP1 94.2(4) 3_666 1_545 ? 
MH2 O13 AP1 105.0(4) . 1_545 ? 
MH1B O14 Si4 143.2(10) . 3_666 ? 
MH1B O14 MH1 21.5(8) . . ? 
Si4 O14 MH1 141.3(7) 3_666 . ? 
MH1B O14 AP2 81.0(12) . 3_656 ? 
Si4 O14 AP2 95.4(9) 3_666 3_656 ? 
MH1 O14 AP2 102.4(9) . 3_656 ? 
MH1B O14 W 88.2(9) . 3_656 ? 
Si4 O14 W 107.9(5) 3_666 3_656 ? 
MH1 O14 W 105.1(5) . 3_656 ? 
AP2 O14 W 31.8(9) 3_656 3_656 ? 
MH1A XM1 MH1 84(6) . . ? 
MH1A XM1 MH1B 108(6) . . ? 
MH1 XM1 MH1B 23.8(7) . . ? 
MH1A XM1 MO4 138(6) . 1_656 ? 
MH1 XM1 MO4 132.0(5) . 1_656 ? 
MH1B XM1 MO4 110.1(8) . 1_656 ? 
MH1A XM1 MO3 78(5) . 1_556 ? 
MH1 XM1 MO3 120.1(4) . 1_556 ? 
MH1B XM1 MO3 123.6(6) . 1_556 ? 
MO4 XM1 MO3 95.2(4) 1_656 1_556 ? 
MH1A XM1 MO5 37(5) . 4_656 ? 
MH1 XM1 MO5 113.2(4) . 4_656 ? 
MH1B XM1 MO5 134.7(8) . 4_656 ? 
MO4 XM1 MO5 101.2(4) 1_656 4_656 ? 
MO3 XM1 MO5 83.7(3) 1_556 4_656 ? 
MH2 XM2 MH2A 23.5(4) . . ? 
MH2 XM2 MO4 130.4(5) . 4_556 ? 
MH2A XM2 MO4 150.2(6) . 4_556 ? 
MH2 XM2 MO2 119.5(4) . 1_556 ? 
MH2A XM2 MO2 112.2(5) . 1_556 ? 
MO4 XM2 MO2 95.1(4) 4_556 1_556 ? 
MH2 XM2 MO5 114.7(5) . 1_556 ? 
MH2A XM2 MO5 92.5(5) . 1_556 ? 
MO4 XM2 MO5 102.2(4) 4_556 1_556 ? 
MO2 XM2 MO5 84.4(3) 1_556 1_556 ? 
MO1 XA1 AP1 134.2(4) 1_566 . ? 
MO1 XA1 MO5 97.6(4) 1_566 3_666 ? 
AP1 XA1 MO5 112.8(4) . 3_666 ? 
MO1 XA1 MO5 96.9(4) 1_566 1_566 ? 
AP1 XA1 MO5 110.6(4) . 1_566 ? 
MO5 XA1 MO5 98.7(3) 3_666 1_566 ? 
MO1 XA2 MO4 98.4(3) . . ? 
MO1 XA2 MO4 98.2(3) . 3 ? 
MO4 XA2 MO4 100.8(3) . 3 ? 
MO1 XA2 AP2 123.0(7) . . ? 
MO4 XA2 AP2 115.0(10) . . ? 
MO4 XA2 AP2 117.5(11) 3 . ? 
MH1 XPM1 MH1B 17.9(5) . . ? 
MH1 XPM1 XPA2 107.1(12) . 1_655 ? 
MH1B XPM1 XPA2 104.7(13) . 1_655 ? 
MH1 XPM1 W 115.7(6) . 1_655 ? 
MH1B XPM1 W 110.1(7) . 1_655 ? 
XPA2 XPM1 W 12.1(7) 1_655 1_655 ? 
MH1 XPM1 XPA1 101.9(6) . 3_666 ? 
MH1B XPM1 XPA1 100.9(6) . 3_666 ? 
XPA2 XPM1 XPA1 150.2(12) 1_655 3_666 ? 
W XPM1 XPA1 139.3(7) 1_655 3_666 ? 
MH1 XPM1 XPA1 98.9(5) . 2_545 ? 
MH1B XPM1 XPA1 116.8(7) . 2_545 ? 
XPA2 XPM1 XPA1 92.0(11) 1_655 2_545 ? 
W XPM1 XPA1 98.6(5) 1_655 2_545 ? 
XPA1 XPM1 XPA1 89.8(6) 3_666 2_545 ? 
MH1 XPM1 W 82.7(5) . 3_656 ? 
MH1B XPM1 W 64.8(7) . 3_656 ? 
XPA2 XPM1 W 90.5(11) 1_655 3_656 ? 
W XPM1 W 83.5(5) 1_655 3_656 ? 
XPA1 XPM1 W 86.8(5) 3_666 3_656 ? 
XPA1 XPM1 W 176.5(6) 2_545 3_656 ? 
MH2 XPM2 MH2A 20.3(3) . . ? 
MH2 XPM2 XPA2 106.6(12) . . ? 
MH2A XPM2 XPA2 106.7(13) . . ? 
MH2 XPM2 XPA1 102.9(6) . 3_666 ? 
MH2A XPM2 XPA1 103.1(6) . 3_666 ? 
XPA2 XPM2 XPA1 149.8(13) . 3_666 ? 
MH2 XPM2 W 116.3(6) . . ? 
MH2A XPM2 W 113.2(6) . . ? 
XPA2 XPM2 W 11.9(9) . . ? 
XPA1 XPM2 W 140.8(7) 3_666 . ? 
MH2 XPM2 XPA2 90.6(10) . 4_556 ? 
MH2A XPM2 XPA2 110.8(10) . 4_556 ? 
XPA2 XPM2 XPA2 87.1(12) . 4_556 ? 
XPA1 XPM2 XPA2 86.5(10) 3_666 4_556 ? 
W XPM2 XPA2 93.8(10) . 4_556 ? 
MH2 XPM2 W 82.5(5) . 4_556 ? 
MH2A XPM2 W 102.8(6) . 4_556 ? 
XPA2 XPM2 W 89.6(12) . 4_556 ? 
XPA1 XPM2 W 88.2(6) 3_666 4_556 ? 
W XPM2 W 97.5(5) . 4_556 ? 
XPA2 XPM2 W 8.1(9) 4_556 4_556 ? 
MH2 XPM2 AP2 139.6(6) . . ? 
MH2A XPM2 AP2 135.6(8) . . ? 
XPA2 XPM2 AP2 33.1(12) . . ? 
XPA1 XPM2 AP2 117.4(7) 3_666 . ? 
W XPM2 AP2 23.5(6) . . ? 
XPA2 XPM2 AP2 89.9(11) 4_556 . ? 
W XPM2 AP2 96.1(8) 4_556 . ? 
AP1 XPA1 XPM2 105.2(6) . 3_666 ? 
AP1 XPA1 XPM1 104.3(6) . 3_666 ? 
XPM2 XPA1 XPM1 150.4(8) 3_666 3_666 ? 
AP1 XPA1 XPM1 94.6(6) . 2_455 ? 
XPM2 XPA1 XPM1 90.4(6) 3_666 2_455 ? 
XPM1 XPA1 XPM1 90.2(6) 3_666 2_455 ? 
W XPA2 AP2 29(5) . . ? 
W XPA2 XPM2 103(6) . . ? 
AP2 XPA2 XPM2 104(2) . . ? 
W XPA2 XPM1 99(6) . 1_455 ? 
AP2 XPA2 XPM1 105.3(19) . 1_455 ? 
XPM2 XPA2 XPM1 150(2) . 1_455 ? 
W XPA2 XPM2 123(7) . 4_556 ? 
AP2 XPA2 XPM2 93(2) . 4_556 ? 
XPM2 XPA2 XPM2 92.9(12) . 4_556 ? 
XPM1 XPA2 XPM2 91.1(15) 1_455 4_556 ? 
XPA2 W AP2 140(7) . . ? 
XPA2 W XPM1 68(6) . 1_455 ? 
AP2 W XPM1 115.6(12) . 1_455 ? 
XPA2 W XPM2 65(6) . . ? 
AP2 W XPM2 112.2(13) . . ? 
XPM1 W XPM2 129.6(7) 1_455 . ? 
XPA2 W O1 93(6) . 4_556 ? 
AP2 W O1 54.4(15) . 4_556 ? 
XPM1 W O1 74.6(5) 1_455 4_556 ? 
XPM2 W O1 125.1(6) . 4_556 ? 
XPA2 W O6 155(6) . 3_556 ? 
AP2 W O6 56.9(17) . 3_556 ? 
XPM1 W O6 87.3(5) 1_455 3_556 ? 
XPM2 W O6 133.6(7) . 3_556 ? 
O1 W O6 87.2(5) 4_556 3_556 ? 
XPA2 W O9 90(6) . 4_556 ? 
AP2 W O9 52.9(17) . 4_556 ? 
XPM1 W O9 122.2(6) 1_455 4_556 ? 
XPM2 W O9 76.4(5) . 4_556 ? 
O1 W O9 52.8(4) 4_556 4_556 ? 
O6 W O9 109.8(6) 3_556 4_556 ? 
XPA2 W O14 147(6) . 3_656 ? 
AP2 W O14 56.6(16) . 3_656 ? 
XPM1 W O14 137.8(6) 1_455 3_656 ? 
XPM2 W O14 82.9(6) . 3_656 ? 
O1 W O14 111.0(6) 4_556 3_656 ? 
O6 W O14 52.6(3) 3_556 3_656 ? 
O9 W O14 87.6(5) 4_556 3_656 ? 
XPA2 W O4 118(6) . 3_566 ? 
AP2 W O4 59.2(11) . 3_566 ? 
XPM1 W O4 57.5(4) 1_455 3_566 ? 
XPM2 W O4 170.5(7) . 3_566 ? 
O1 W O4 47.5(3) 4_556 3_566 ? 
O6 W O4 46.9(3) 3_556 3_566 ? 
O9 W O4 94.5(5) 4_556 3_566 ? 
O14 W O4 94.3(5) 3_656 3_566 ? 
XPA2 W O11 112(6) . . ? 
AP2 W O11 56.6(11) . . ? 
XPM1 W O11 169.0(7) 1_455 . ? 
XPM2 W O11 56.0(4) . . ? 
O1 W O11 94.4(5) 4_556 . ? 
O6 W O11 93.4(5) 3_556 . ? 
O9 W O11 47.4(3) 4_556 . ? 
O14 W O11 47.0(3) 3_656 . ? 
O4 W O11 115.8(6) 3_566 . ? 
XM1 MH1A MO5 128(7) . 4_656 ? 
XM1 MH1A MH1 70(5) . . ? 
MO5 MH1A MH1 143(4) 4_656 . ? 
XM1 MH1A MO3 81(5) . 1_556 ? 
MO5 MH1A MO3 100(3) 4_656 1_556 ? 
MH1 MH1A MO3 116(3) . 1_556 ? 
XM1 MH1A MH1B 52(5) . . ? 
MO5 MH1A MH1B 151(4) 4_656 . ? 
MH1 MH1A MH1B 18.1(10) . . ? 
MO3 MH1A MH1B 108(3) 1_556 . ? 
XM1 MH1A O2 109(6) . . ? 
MO5 MH1A O2 123(4) 4_656 . ? 
MH1 MH1A O2 50.3(19) . . ? 
MO3 MH1A O2 93(2) 1_556 . ? 
MH1B MH1A O2 64(2) . . ? 
XM1 MH1A O8 104(6) . 1_655 ? 
MO5 MH1A O8 93(3) 4_656 1_655 ? 
MH1 MH1A O8 49.8(18) . 1_655 ? 
MO3 MH1A O8 158(3) 1_556 1_655 ? 
MH1B MH1A O8 63(2) . 1_655 ? 
O2 MH1A O8 65(2) . 1_655 ? 
XM1 MH1A MO4 31(4) . 1_656 ? 
MO5 MH1A MO4 97(3) 4_656 1_656 ? 
MH1 MH1A MO4 97(3) . 1_656 ? 
MO3 MH1A MO4 79(2) 1_556 1_656 ? 
MH1B MH1A MO4 80(2) . 1_656 ? 
O2 MH1A MO4 139(3) . 1_656 ? 
O8 MH1A MO4 116(3) 1_655 1_656 ? 
XM1 MH1A MO2 78(5) . 1_656 ? 
MO5 MH1A MO2 57.8(17) 4_656 1_656 ? 
MH1 MH1A MO2 104(3) . 1_656 ? 
MO3 MH1A MO2 124(3) 1_556 1_656 ? 
MH1B MH1A MO2 98(2) . 1_656 ? 
O2 MH1A MO2 143(3) . 1_656 ? 
O8 MH1A MO2 77.4(16) 1_655 1_656 ? 
MO4 MH1A MO2 57.4(13) 1_656 1_656 ? 
MH1 MH1B O6 117.0(17) . 1_655 ? 
MH1 MH1B O14 109.2(17) . . ? 
O6 MH1B O14 127.9(16) 1_655 . ? 
MH1 MH1B XM1 71.1(15) . . ? 
O6 MH1B XM1 108.2(11) 1_655 . ? 
O14 MH1B XM1 108.5(11) . . ? 
MH1 MH1B MH1A 51(2) . . ? 
O6 MH1B MH1A 116(2) 1_655 . ? 
O14 MH1B MH1A 111.7(19) . . ? 
XM1 MH1B MH1A 20(2) . . ? 
MH1 MH1B XPM1 70.1(14) . . ? 
O6 MH1B XPM1 86.8(10) 1_655 . ? 
O14 MH1B XPM1 87.2(9) . . ? 
XM1 MH1B XPM1 141.1(12) . . ? 
MH1A MH1B XPM1 121(2) . . ? 
MH1 MH1B O8 34.2(10) . 1_655 ? 
O6 MH1B O8 82.9(9) 1_655 1_655 ? 
O14 MH1B O8 139.8(12) . 1_655 ? 
XM1 MH1B O8 79.1(8) . 1_655 ? 
MH1A MH1B O8 63(2) . 1_655 ? 
XPM1 MH1B O8 67.2(6) . 1_655 ? 
MH1 MH1B O2 31.3(10) . . ? 
O6 MH1B O2 145.0(12) 1_655 . ? 
O14 MH1B O2 77.9(8) . . ? 
XM1 MH1B O2 79.1(8) . . ? 
MH1A MH1B O2 62(2) . . ? 
XPM1 MH1B O2 69.5(7) . . ? 
O8 MH1B O2 64.6(6) 1_655 . ? 
MH1 MH1B AP2 172.1(19) . 3_656 ? 
O6 MH1B AP2 65.5(10) 1_655 3_656 ? 
O14 MH1B AP2 65.7(10) . 3_656 ? 
XM1 MH1B AP2 115.7(12) . 3_656 ? 
MH1A MH1B AP2 136(2) . 3_656 ? 
XPM1 MH1B AP2 103.1(11) . 3_656 ? 
O8 MH1B AP2 147.7(9) 1_655 3_656 ? 
O2 MH1B AP2 143.3(9) . 3_656 ? 
MH1 MH1B Si2 116.8(14) . 1_655 ? 
O6 MH1B Si2 17.9(6) 1_655 1_655 ? 
O14 MH1B Si2 133.8(12) . 1_655 ? 
XM1 MH1B Si2 90.9(7) . 1_655 ? 
MH1A MH1B Si2 100.9(18) . 1_655 ? 
XPM1 MH1B Si2 103.6(7) . 1_655 ? 
O8 MH1B Si2 83.9(5) 1_655 1_655 ? 
O2 MH1B Si2 148.1(8) . 1_655 ? 
AP2 MH1B Si2 68.1(7) 3_656 1_655 ? 
MH1 MH1B Si4 111.1(14) . 3_666 ? 
O6 MH1B Si4 131.6(12) 1_655 3_666 ? 
O14 MH1B Si4 18.5(5) . 3_666 ? 
XM1 MH1B Si4 91.4(7) . 3_666 ? 
MH1A MH1B Si4 98.1(18) . 3_666 ? 
XPM1 MH1B Si4 105.3(7) . 3_666 ? 
O8 MH1B Si4 145.3(8) 1_655 3_666 ? 
O2 MH1B Si4 80.9(5) . 3_666 ? 
AP2 MH1B Si4 66.1(7) 3_656 3_666 ? 
Si2 MH1B Si4 130.0(8) 1_655 3_666 ? 
MH1 MH1B W 144.8(18) . 3_656 ? 
O6 MH1B W 63.7(9) 1_655 3_656 ? 
O14 MH1B W 64.7(9) . 3_656 ? 
XM1 MH1B W 144.0(11) . 3_656 ? 
MH1A MH1B W 164(2) . 3_656 ? 
XPM1 MH1B W 74.9(7) . 3_656 ? 
O8 MH1B W 130.3(8) 1_655 3_656 ? 
O2 MH1B W 128.9(7) . 3_656 ? 
AP2 MH1B W 28.2(8) 3_656 3_656 ? 
Si2 MH1B W 74.9(6) 1_655 3_656 ? 
Si4 MH1B W 74.4(5) 3_666 3_656 ? 
MH2 MH2A O5 112.9(11) . . ? 
MH2 MH2A O13 112.2(10) . . ? 
O5 MH2A O13 133.7(10) . . ? 
MH2 MH2A XM2 59.6(8) . . ? 
O5 MH2A XM2 106.7(8) . . ? 
O13 MH2A XM2 104.7(8) . . ? 
MH2 MH2A XPM2 75.5(9) . . ? 
O5 MH2A XPM2 89.5(8) . . ? 
O13 MH2A XPM2 91.7(8) . . ? 
XM2 MH2A XPM2 135.2(7) . . ? 
MH2 MH2A O9 34.3(6) . . ? 
O5 MH2A O9 79.0(6) . . ? 
O13 MH2A O9 143.0(8) . . ? 
XM2 MH2A O9 74.0(5) . . ? 
XPM2 MH2A O9 68.4(5) . . ? 
MH2 MH2A AP1 172.3(12) . 1_545 ? 
O5 MH2A AP1 67.6(6) . 1_545 ? 
O13 MH2A AP1 66.3(6) . 1_545 ? 
XM2 MH2A AP1 128.0(6) . 1_545 ? 
XPM2 MH2A AP1 96.8(6) . 1_545 ? 
O9 MH2A AP1 143.8(5) . 1_545 ? 
MH2 MH2A Si2 116.9(9) . . ? 
O5 MH2A Si2 11.7(5) . . ? 
O13 MH2A Si2 130.9(7) . . ? 
XM2 MH2A Si2 98.8(5) . . ? 
XPM2 MH2A Si2 101.2(5) . . ? 
O9 MH2A Si2 84.8(4) . . ? 
AP1 MH2A Si2 65.2(3) 1_545 . ? 
MH2 MH2A Si4 115.0(8) . 3_666 ? 
O5 MH2A Si4 132.2(8) . 3_666 ? 
O13 MH2A Si4 11.2(5) . 3_666 ? 
XM2 MH2A Si4 96.4(5) . 3_666 ? 
XPM2 MH2A Si4 102.9(5) . 3_666 ? 
O9 MH2A Si4 148.5(5) . 3_666 ? 
AP1 MH2A Si4 65.2(3) 1_545 3_666 ? 
Si2 MH2A Si4 126.6(4) . 3_666 ? 
MH2 MH2A MO5 106.2(10) . 1_556 ? 
O5 MH2A MO5 101.7(7) . 1_556 ? 
O13 MH2A MO5 75.3(6) . 1_556 ? 
XM2 MH2A MO5 48.5(4) . 1_556 ? 
XPM2 MH2A MO5 166.6(5) . 1_556 ? 
O9 MH2A MO5 120.6(5) . 1_556 ? 
AP1 MH2A MO5 80.9(3) 1_545 1_556 ? 
Si2 MH2A MO5 89.9(3) . 1_556 ? 
Si4 MH2A MO5 64.1(3) 3_666 1_556 ? 
MH2 MH2A MO2 77.9(8) . 1_556 ? 
O5 MH2A MO2 70.9(6) . 1_556 ? 
O13 MH2A MO2 129.5(8) . 1_556 ? 
XM2 MH2A MO2 35.9(3) . 1_556 ? 
XPM2 MH2A MO2 137.3(5) . 1_556 ? 
O9 MH2A MO2 70.7(4) . 1_556 ? 
AP1 MH2A MO2 109.0(4) 1_545 1_556 ? 
Si2 MH2A MO2 62.9(2) . 1_556 ? 
Si4 MH2A MO2 118.5(4) 3_666 1_556 ? 
MO5 MH2A MO2 54.9(2) 1_556 1_556 ? 
MH2 MH2A W 86.3(9) . . ? 
O5 MH2A W 53.2(6) . . ? 
O13 MH2A W 120.7(8) . . ? 
XM2 MH2A W 131.5(6) . . ? 
XPM2 MH2A W 37.0(4) . . ? 
O9 MH2A W 59.8(4) . . ? 
AP1 MH2A W 88.1(4) 1_545 . ? 
Si2 MH2A W 64.9(3) . . ? 
Si4 MH2A W 130.7(5) 3_666 . ? 
MO5 MH2A W 154.9(4) 1_556 . ? 
MO2 MH2A W 108.9(4) 1_556 . ? 
 
_diffrn_measured_fraction_theta_max    0.975 
_diffrn_reflns_theta_full              30.06 
_diffrn_measured_fraction_theta_full   0.975 
_refine_diff_density_max    3.262 
_refine_diff_density_min   -1.643 
_refine_diff_density_rms    0.304 
